Supramolecular isomerism and structural flexibility in coordination networks sustained by cadmium rod building blocks.
Andaloussi, Yassin H.; Bezrukov, Andrey A.; Sensharma, Debobroto; Zaworotko, Michael J.; CrystEngComm 25 (2023) 4175–4181; doi:10.1039/d3ce00557g

data_7246975
_publ_section_title
;
 Supramolecular isomerism and structural flexibility in coordination
 networks sustained by cadmium rod building blocks.
;
_journal_issue                   29
_journal_name_full               CrystEngComm
_journal_page_first              4175
_journal_page_last               4181
_journal_paper_doi               10.1039/d3ce00557g
_journal_volume                  25
_journal_year                    2023
_chemical_formula_moiety         'C20 H14 Cd N4 O8'
_chemical_formula_sum            'C20 H14 Cd N4 O8'
_chemical_formula_weight         550.75
_chemical_name_common            Cd(PyImPr)2-hlz-beta
_chemical_name_systematic
Catena-[bis(\b-(3,4-pyridinedicarboximido)propionato)-cadmium]
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2022-01-10
_audit_creation_method
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_audit_update_record
;
2023-02-24 deposited with the CCDC.	2023-07-03 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 97.893(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.9218(2)
_cell_length_b                   18.3280(7)
_cell_length_c                   10.9159(5)
_cell_measurement_reflns_used    9952
_cell_measurement_temperature    100.15
_cell_measurement_theta_max      72.68
_cell_measurement_theta_min      2.41
_cell_volume                     975.36(7)
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL  (Sheldrick, 2008)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      100.15
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0534
_diffrn_reflns_av_unetI/netI     0.0295
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            14024
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         72.676
_diffrn_reflns_theta_min         4.748
_diffrn_source_current           1.0
_diffrn_source_power             0.05
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    9.521
_exptl_absorpt_correction_T_max  0.7536
_exptl_absorpt_correction_T_min  0.4016
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1521 before and 0.0975 after correction.
The Ratio of minimum to maximum transmission is 0.5329.
The \l/2 correction factor is Not present.
;
_exptl_crystal_colour            'dull colourless'
_exptl_crystal_colour_lustre     dull
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.875
_exptl_crystal_description       block
_exptl_crystal_F_000             548
_exptl_crystal_recrystallization_method
'Reactive crystallisation (Solvothermal)'
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.11
_refine_diff_density_max         1.502
_refine_diff_density_min         -0.851
_refine_diff_density_rms         0.165
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.323
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         1915
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.323
_refine_ls_R_factor_all          0.0773
_refine_ls_R_factor_gt           0.0757
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+14.2889P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1779
_refine_ls_wR_factor_ref         0.1785
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1845
_reflns_number_total             1915
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d3ce00557g2.cif
_cod_data_source_block           Cd(PyImPr)2-hlz-beta
_cod_depositor_comments
'Adding full bibliography for 7246974--7246977.cif.'
_cod_database_code               7246975
_shelx_shelxl_version_number     2014/7
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
2.a Secondary CH2 refined with riding coordinates:
 C9(H9A,H9B), C8(H8A,H8B)
2.b Aromatic/amide H refined with riding coordinates:
 C5(H5), C1(H1), C4(H4)
;
_shelx_res_checksum              49285
_olex2_submission_special_instructions 'No special instructions were received'